A 249/A 249M – 043. Ordering Information 3.1.4 Size (outside diameter and nominal wall thickness), 3.1 It is the responsibility of the purchaser to specify all 3.1.5 Length (speciﬁc or random),requirements that are necessary for material ordered under this 3.1.6 Optional requirements (13.6),speciﬁcation. Such requirements may include, but are not 3.1.7 Test report required (see Certiﬁcation Section oflimited to, the following: Speciﬁcation A 1016/A 1016M), 3.1.1 Quantity (feet, metres, or number of lengths), 3.1.2 Name of material welded tubes (WLD) or heavily cold 3.1.8 Speciﬁcation designation, andworked tubes (HCW), 3.1.9 Special requirements and any supplementary require- 3.1.3 Grade (Table 1), ments selected. 2
TABLE 1 Continued Composition, % Grade UNS Carbon Manganese Phosphorous Sulfur Silicon Chromium Nickel Molybdenum NitrogenC Copper Other DesignationB ... S31725 0.030 2.00 0.045 0.030 1.00 18.0–20.0 13.5–17.5 4.0–5.0 0.20 ... ... ... S31726 0.030 2.00 0.045 0.030 1.00 17.0–20.0 14.5–17.5 4.0–5.0 0.10–0.20 ... ... ... S32050 0.030 1.50 0.035 0.020 1.00 22.0–24.0 20.0–23.0 6.0–6.8 0.21–0.32 0.40 ... TP321 S32100 0.08 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... 0.10 ... Ti 5(C+N)- 0.70 TP321H S32109 0.04–0.10 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... 0.10 ... Ti 5(C+N)- 0.70 ... S32654 0.020 2.0–4.0 0.030 0.005 0.50 24.0–25.0 21.0–23.0 7.0–8.0 0.45–0.55 0.30–0.60 ... ... S33228 0.04–0.08 1.00 0.020 0.015 0.30 26.0–28.0 31.0–333.0 ... ... ... Cb 0.60–1.00 Ce 0.05–0.10 Al0.025 ... S34565 0.030 5.0–7.0 0.030 0.010 1.00 23.0–25.0 16.0–18.0 4.0–5.0 0.40–0.60 ... Cb 0.10 TP347 S34700 0.08 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... ... ... Cb 10xC- 1.10 TP347H S34709 0.04–0.10 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... ... ... Cb 8xC- 1.105 TP348 S34800 0.08 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... ... ... (Cb+Ta) 10xC-1.10 Ta 0.10 Co 0.20 TP348H S34809 0.04–0.10 2.00 0.045 0.030 1.00 17.0–19.0 9.0–12.0 ... ... ... (Cb+Ta) 8xC-1.10 Ta 0.10 A 249/A 249M – 04 Co 0.20 ... S35045 0.06–0.10 1.50 0.045 0.015 1.00 25.0–29.0 32.0–37.0 ... ... 0.75 Al 0.15–0.60 Ti 0.15–0.60 TPXM-15 S38100 0.08 2.00 0.030 0.030 1.50–2.50 17.0–19.0 17.5–18.5 ... ... ... ... ... S38815 0.030 2.00 0.040 0.020 5.5–6.5 13.0–15.0 15.0–17.0 0.75–1.50 ... 0.75–1.50 Al 0.30 max ... N08367 0.030 2.00 0.040 0.030 1.00 20.0–22.0 23.5–25.5 6.0–7.0 0.18–0.25 0.75 ... ... N08926 0.020 2.00 0.030 0.010 0.50 19.0–21.0 24.0–26.0 6.0–7.0 0.15–0.25 0.50–1.50 ... ... N08904 0.020 2.00 0.040 0.030 1.00 19.0–23.0 23.0–28.0 4.0–5.0 0.10 1.00–2.00 ... A Maximum, unless otherwise indicated. B New designation established in accordance with Practice E 527 and SAE J1086, Practice for Numbering Metals and Alloys (UNS). C The method of analysis for nitrogen shall be a matter of agreement between the purchaser and manufacturer. D For small diameter or thin walls, or both, where many drawing passes are required, a carbon maximum of 0.040 % is necessary in Grades TP 304L and TP 316L. Small outside diameter tubes are deﬁned as those less than 0.500 in. [12.7 mm] in outside diameter and light wall are those less than 0.049 in. [1.2 mm] in minimum wall thickness.
A 249/A 249M – 044. General Requirements 6.2 A solution annealing temperature above 1950°F 4.1 Material furnished under this speciﬁcation shall con- [1065°C] may impair the resistance to intergranular corrosionform to the applicable requirements of the current edition of after subsequent exposure to sensitizing conditions inSpeciﬁcation A 1016/A 1016M, unless otherwise provided TP309HCb, TP310HCb, TP321, TP321H, TP347, TP347H,herein. TP348, and TP348H. When speciﬁed by the purchaser, a lower temperature stabilization or re-solution anneal shall be used5. Manufacture subsequent to the initial high temperature solution anneal (see Supplementary Requirement S4). 5.1 The welded (WLD) tubes shall be made from ﬂat-rolledsteel by an automatic welding process with no addition of ﬁller 7. Chemical Compositionmetal. 5.1.1 Subsequent to welding and prior to ﬁnal heat treat- 7.1 The heat analysis shall conform to the requirements asment, the tubes shall be cold worked either in both weld and to chemical composition given in Table 1.base metal or in weld metal only. The method of cold workingmay be speciﬁed by the purchaser. When cold drawn, the 8. Product Analysispurchaser may specify the minimum amount of reduction in 8.1 An analysis of either one length of ﬂat-rolled stock orcross-sectional area or wall thickness, or both. one tube shall be made for each heat. The chemical composi- 5.1.2 Heavily cold worked (HCW) tubes shall be made by tion thus determined shall conform to the requirements given inapplying cold working of not less than 35 % reduction in both Section 7.wall and weld to a welded tube prior to the ﬁnal anneal. No 8.2 A product analysis tolerance of Table A1.1 in Speciﬁ-ﬁller metal shall be used in the making of the weld. Prior to cation A 480/A 480M shall apply. The product analysis toler-cold working, the weld shall be 100 % radiographically in- ance is not applicable to the carbon content for material with aspected in accordance with the requirements of ASME Boiler speciﬁed maximum carbon of 0.04 % or less.and Pressure Vessel Code, Section VIII, Division 1, latest 8.3 If the original test for product analysis fails, retests ofrevision, Paragraph UW 51. two additional lengths of ﬂat-rolled stock or tubes shall be made. Both retests for the elements in question shall meet the6. Heat Treatment requirements of the speciﬁcation; otherwise all remaining 6.1 All material shall be furnished in the heat-treated material in the heat or lot (Note 1) shall be rejected or, at thecondition in accordance with the requirements of Table 2. option of the producer, each length of ﬂat-rolled stock or tube TABLE 2 Heat Treatment Requirements Grade UNS Number Solutioning Temperature, min or range Quenching Method A All grades not 1900°F [1040°C] individually listed below B ... S30815 1920°F [1050°C] TP309HCb S30941 1900°F [1040°C]C B B TP310H S31009 1900°F [1040°C] TP310HCb S31041 1900°F [1040°C]C B B ... S31254 2100°F [1150°C] B TP316H S31609 1900°F [1040°C] TP321 S32100 1900°F [1040°C]C B TP321H S32109 2000°F [1100°C]C B B ... S32654 2100°F [1150°C] B ... S33228 2050°F [1120°C] B ... S34565 2050°F [1120°C]– B 2140°F [1170°C] TP347 S34700 1900°F [1040°C]C B TP347H S34709 2000°F [1100°C]C B TP348 S34800 1900°F [1040°C]C B TP348H S34809 2000°F [1100°C]C B D ... S35045 2000°F [1100°C] B ... S38815 1950°F [1065°C] B ... N08367 2025°F [1110°C] B ... N08904 2000°F [1100°C] B ... N08926 2010°F [1105°C] A Quenched in water or rapidly cooled by other methods, at a rate sufficient to prevent reprecipitation of carbides, as demonstrated by the capability of passing PracticesA 262, Practice E. The manufacturer is not required to run the test unless it is speciﬁed on the purchase order (See Supplementary Requirement S6). Note that PracticesA 262 requires the test to be performed on sensitized specimens in the low carbon and stabilized types and on specimens representative of the as-shipped condition ofthe other types. In the case of low-carbon types containing 3 % or more molybdenum, the applicability of the sensitizing treatment prior to testing shall be a matter fornegotiation between the seller and purchaser. B Quenched in water or rapidly cooled by other methods. C A solution treating temperature above 1950°F [1065°C] may impair resistance to intergranular corrosion after subsequent exposure to sensitizing conditions in theindicated grades. When speciﬁed by the purchaser, a lower temperature stabilization or re-solution anneal shall be used subsequent to the higher-temperature solutionanneal prescribed in this table (See Supplementary Requirement S4). D Cooled in still air, or faster. 6
A 249/A 249M – 04may be individually tested for acceptance. Lengths of ﬂat- TABLE 4 Tensile and Hardness RequirementsArolled stock or tubes that do not meet the requirements of the Grade UNS Tensile Yield Elongation Rockwellspeciﬁcation shall be rejected. Designation Strength, Strength, in 2 in. or Hardness min, ksi min, ksi 50 mm, Number, [MPa] [MPa] min, % max NOTE 1—For ﬂattening and ﬂange requirements, the term lot applies toall tubes prior to cutting of the same nominal size and wall thickness TP201 S20100 95  38  35 B95which are produced from the same heat of steel. When ﬁnal heat treatment TP202 S20200 90  38  35 B95 TPXM-19 S20910 100  55  35 C25is in a batch-type furnace, a lot shall include only those tubes of the same TPXM-29 S24000 100  55  35 B100size and from the same heat which are heat treated in the same furnace ... S24565 115  60  35 B100charge. When the ﬁnal heat treatment is in a continuous furnace, the TP304 S30400 75  30  35 B90number of tubes of the same size and from the same heat in a lot shall be TP304L S30403 70  25  35 B90determined from the size of the tubes as prescribed in Table 3. TP304H S30409 75  30  35 B90 ... S30415 87  42  35 B96 NOTE 2—For tension and hardness test requirements, the term lot TP304N S30451 80  35  35 B90applies to all tubes prior to cutting, of the same nominal diameter and wall TP304LN S30453 75  30  35 B90thickness which are produced from the same heat of steel. When ﬁnal heat TP305 S30500 75  30  35 B90treatment is in a batch-type furnace, a lot shall include only those tubes of ... S30615 90  40  35 B95the same size and the same heat which are heat treated in the same furnace ... S30815 87  45  35 B95charge. When the ﬁnal heat treatment is in a continuous furnace, a lot shall TP309S S30908 75  30  35 B90 TP309H S30909 75  30  35 B90include all tubes of the same size and heat, annealed in the same furnace TP309Cb S30940 75  30  35 B90at the same temperature, time at heat, and furnace speed. TP309HCb S30941 75  30  35 B90 TP310S S31008 75  30  35 B909. Tensile Requirements TP310H S31009 75  30  35 B90 TP310Cb S31040 75  30  35 B90 9.1 The material shall conform to the tensile properties TP310HCb S31041 75  30  35 B90prescribed in Table 4. ... S31050: t # 0.25 in. 84  39  25 B95 t > 0.25 in. 78  37  25 B9510. Hardness Requirements ... S31254: t # 0.187 in. 98  45  35 B100 10.1 The tubes shall have a Rockwell hardness number not [5.00 mm]exceeding the values speciﬁed in Table 4. t > 0.187 in. 95  45  35 B100 [5.00 mm] TP316 S31600 75  30  35 B9011. Reverse-Bend Test Requirement TP316L S31603 70  25  35 B90 TP316H S31609 75  30  35 B90 11.1 A section 4 in. [100 mm] minimum in length shall be TP316N S31651 80  35  35 B90split longitudinally 90° on each side of the weld. The sample TP316LN S31653 75  30  35 B90 TP317 S31700 75  30  35 B90shall then be opened and bent around a mandrel with a TP317L S31703 75  30  35 B90maximum thickness of four times the wall thickness, with the ... S31725 75  30  35 B90mandrel parallel to the weld and against the original outside ... S31726 80  35  35 B90 ... S32050 98  48  40surface of the tube. The weld shall be at the point of maximum TP321 S32100 75  30  35 B90bend. There shall be no evidence of cracks, or of overlaps TP321H S32109 75  30  35 B90resulting from the reduction in thickness of the weld areas by ... S32654 109  62  35 B100 ... S33228 73  27  30 B90cold working. When the geometry or size of the tubing make it TP347 S34700 75  30  35 B90difficult to test the sample as a single piece, the sample may be TP347H S34709 75  30  35 B90sectioned into smaller pieces provided a minimum of 4 in. of TP348 S34800 75  30  35 B90 TP348H S34809 75  30  35 B90weld is subjected to reverse bending. ... S35045 70  25  35 B90 TPXM-15 S38100 75  30  35 B90 NOTE 3—The reverse bend test is not applicable when the speciﬁed ... S38815 78  37  30 B100wall is 10 % or more of the speciﬁed outside diameter, or the wall ... N08367thickness is 0.134 in. [3.4 mm] or greater, or the outside diameter size is t # 0.187 100  45  30 100less than 0.375 in. [9.5 mm]. Under these conditions the reverse ﬂattening t > 0.187 95  45  30 100 ... N08904 71  31  35 B90test of Speciﬁcation A 1016/A 1016M shall apply. ... N08926 94  43  35 B100 A Not applicable to tubes less than 1⁄8 in. [3.2 mm] in outside diameter or having wall thickness below 0.015 in. [0.4 mm], or both. The tensile properties of such TABLE 3 Number of Tubes in a Lot Heat Treated by the small diameter or thin wall tubes shall be a matter of agreement between the Continuous Process manufacturer and the purchaser. Size of Tube Size of Lot 2 in. [50.8 mm] and over in outside not more than 50 tubes diameter and 0.200 in. [5.1 mm] and over 12. Grain Size Requirement in wall thickness 12.1 The grain size of Grades TP309H, TP309HCb, Less than 2 in. [50.8 mm] but over 1 in. not more than 75 tubes [25.4 mm] in outside diameter or over 1 in. TP310H and TP310HCb, as determined in accordance with [25.4 mm] in outside diameter and under Test Methods E 112, shall be No. 6 or coarser. 0.200 in. [5.1 mm] in wall thickness 12.2 The grain size of Grades TP304H, TP316H, TP321H, 1 in. [25.4 mm] or less in outside diameter not more than 125 tubes TP347H and TP348H, as determined in accordance with Test Methods E 112, shall be No. 7 or coarser. 7
A 249/A 249M – 0413. Mechanical Tests and Grain Size Determinations 14.2.1 Requirements of 14.2 are not applicable when any of Required the following apply: 13.1 Tension Test—One tension test shall be made on a 188.8.131.52 When the speciﬁed wall thickness exceeds 12 % ofspecimen for lots of not more than 50 tubes. Tension tests shall the speciﬁed outside diameter;be made on specimens from two tubes for lots of more than 50 184.108.40.206 When the speciﬁed wall thickness exceeds 0.165tubes (Note 2). in. [4.2 mm]; 13.2 Flattening Test—One ﬂattening test shall be made on 220.127.116.11 When the speciﬁed OD exceeds 3 in. [76.2 mm]; orspecimens from each end of one ﬁnished tube, not the one used 18.104.22.168 When the speciﬁed minimum yield strength givenfor the ﬂange test, from each lot (Note 1). in Table 4 for the speciﬁed grade is 35 ksi [240 MPa] or greater. 13.3 Flange Test—One ﬂange test shall be made on speci- 15. Workmanship, Finish, and Appearancemens from each end of one ﬁnished tube, not the one used forthe ﬂattening test, from each lot (Note 1). 15.1 Finished tubes shall have smooth ends free of burrs and 13.4 Reverse-Bend Test—One reverse-bend test shall be shall not deviate from straightness by more than 0.030 in. [0.8made on a specimen from each 1500 ft [450 m] of ﬁnished mm] in 3 ft (900 mm] of length.tubing. 16. Surface Condition 13.5 Hardness Test—Brinell or Rockwell hardness testsshall be made on specimens from two tubes from each lot 16.1 The tubes, after ﬁnal heat treatment, shall be chemi-(Note 2). cally descaled or pickled free of scale. When bright annealing 13.6 Hydrostatic or Nondestructive Electric Test—Each is used, pickling or chemical descaling is not necessary.tube shall be subjected to either the hydrostatic or the nonde-structive electric test. The purchaser may specify which test is 17. Forming Operationsto be used. 17.1 Tubes when inserted in the boiler shall stand expanding 13.7 Grain Size—Grain size determinations on grades and beading without showing cracks or ﬂaws. All tubes, whenTP309H, TP309HCb, TP310H and TP310HCb shall be made properly manipulated, shall be able to stand expanding andon the same number of tubes as prescribed for the ﬂattening beading without showing cracks and ﬂaws, and also shall standtest. all forging, welding, and bending operations necessary for 13.8 Heavily cold worked tubes (HCW) shall be capable of application without developing defects.passing the weld decay test listed in Supplementary S7 with aweld metal to base metal loss ratio of 0.90 to 1.10. The test is 18. Product Markingnot required unless S7 is speciﬁed in the purchase order. 18.1 In addition to the marking prescribed in Speciﬁcation A 1016/A 1016M, the marking for Grades TP304H, TP309H,14. Permissible Variations in Dimensions TP309HCb, TP310H, TP310HCb, TP316H, TP321H, TP347H, 14.1 Dimensional tolerances other than wall thickness tol- and TP348H shall also include the heat number and theerances shall be in accordance with Speciﬁcation A 1016/ heat-treatment lot identiﬁcation.A 1016M. Wall thickness tolerances shall be 610 % of nomi-nal wall for all tubing sizes. 19. Keywords 14.2 The wall thickness of the weld shall not exceed the 19.1 austenitic stainless steel; boiler tubes; condenser tube;wall thickness measured 90° from the weld by more than 6 % heat exchanger tube; high temperature applications; steel tube;of the speciﬁed wall thickness or 0.004 in. [0.1 mm], which- superheater tubes; temperature service applications, high;ever is greater. welded steel tube and heavily cold worked (HCW) tubes SUPPLEMENTARY REQUIREMENTS The following supplementary requirements shall apply only when speciﬁed by the purchaser in the inquiry, contract, or order.S1. Stress-Relieved Annealed Tubes S1.2 When stress-relieved tubes are speciﬁed, tubes shall be S1.1 For use in certain corrosives, particularly chlorides given a heat treatment at 1550 to 1650°F [845 to 900°C] afterwhere stress corrosion may occur, tubes in Grades TP304L, roll straightening. Cooling from this temperature range may beTP316L, TP321, TP347, and TP348 may be speciﬁed in the either in air or by slow cooling. No mechanical straightening isstress-relieved annealed condition. Details of these supplemen- permitted after the stress-relief treatment.tal requirements shall be agreed upon by the manufacturer and S1.3 Straightness of the tubes shall be a matter of negotiationthe purchaser. between the purchaser and manufacturer. 8
A 249/A 249M – 04S2. Minimum Wall Tubes of the tube opposite the weld consisting of 100 % base metal. S2.1 When speciﬁed by the purchaser, tubes shall be fur- Remove all burrs and sharp edges by lightly grinding. Removenished on a minimum wall basis. Such tubes shall satisfy the dust and grease by cleaning with soap and water or otherminimum wall thickness requirements of Speciﬁcation A 1016/ suitable solvents. Then, place sample(s) in the ﬂask. It is notA 1016M rather than the nominal wall requirements of this recommended to test more than four samples together, or tospeciﬁcation. In addition to the marking required by Section mix alloy types.18, the tubing shall be marked S2. S7.4 Prepare the hydrochloric acid solution by slowly add- ing reagent grade (approximately 37 %) hydrochloric acid toS3. Air Underwater Pressure Test an equal volume of distilled water. (Warning—Protect eyes S3.1 When speciﬁed, the tubing shall be examined by the air and use rubber gloves when handling acid. Mixing shall beunderwater pressure test. done under a hood and testing shall be run under a hood.) S7.5 The test container shall be a 1-L Erlenmeyer ﬂaskS4. Stabilizing Heat Treatment equipped with ground-glass joints and an Ahlin condenser. The S4.1 Subsequent to the solution anneal required in Section volume of the solution shall be approximately 700 mL.6, Grades TP309HCb, TP310HCb, TP321, TP321H, TP347, S7.6 Measure the thickness of the tube at ﬁve locationsTP347H, TP348, and TP348H shall be given a stabilization along the weld area and at ﬁve locations along the base-metalheat treatment at a temperature lower than that used for the section. In both cases, take measurements at approximatelyinitial solution annealing heat treatment. The temperature of equal longitudinal intervals along the section lengths. Makestabilization heat treatment shall be at a temperature as agreed these measurements with a sharp pointed micrometer accurateupon between the purchaser and vendor. to at least 0.001 in. The micrometer must be suitable for measuring the small features in the surface after testing.S5. Unstraightened Tubes Typical pin micrometers have tapered anvils with a tip radius S5.1 When the purchaser speciﬁes tubes unstraightened of less than 0.015 in.after ﬁnal heat treatment (such as coils), the straightness S7.7 Immerse the samples into the solution. Add boilingrequirement of Section 12 shall not apply and the minimum chips and bring to a boil. Allow the chips to remain boilingyield strength of Table 3 shall be reduced by 5 ksi [35 MPa]. throughout the test. The time of testing shall be that which is S5.2 On the certiﬁcation, and wherever the grade designa- required to remove 40 to 60 % of the original base-metaltion for unstraightened tubing appears, it shall be identiﬁed thickness (usually 2 h or less). If more than 60 % of thewith the suffix letter “U” (for example, 304-U, 321-U, etc.). base-metal thickness remains, the sample may be removed after 24 h.S6. Intergranular Corrosion Test S7.8 At the end of the test period, remove the samples from S6.1 When speciﬁed, material shall pass intergranular cor- the solution, rinse with distilled water, and dry.rosion tests conducted by the manufacturer in accordance with S7.9 After exposure to the test solution, repeat the tube-Practices A 262, Practice E. thickness measurement as in S7.6. If the thinning is not uniform across the width of the weld, then two sets of NOTE S6.1—Practice E requires testing on the sensitized condition for weld-metal measurement are required. One set of measure-low carbon or stabilized grades, and on the as-shipped condition for other ments is to be taken along the centerline of the weld. Thegrades. second set of measurements is to be taken in the thinnest area S6.2 A stabilization heat treatment in accordance with of the weld.Supplementary Requirement S4 may be necessary and is S7.10 Calculate the corrosion ratio, R, for both sections ofpermitted in order to meet this requirement for the grades the weld as follows in Eq 1:containing titanium or columbium, particularly in their H Wo 2 Wversions. R5 B 2B (1) oS7. Weld Decay Test where: S7.1 This test is not applicable to alloys with a nickel Wo = average weld-metal thickness before the test,content $ 19.0 % or a molybdenum content $ 4.00 %, or both. W = average weld-metal thickness after the test, S7.2 When speciﬁed by the purchase order, one sample Bo = average base-metal thickness before the test, andfrom each lot of tubing (Note 2) shall be subjected to testing in B = average base-metal thickness after the test.a boiling mixture of 50 % reagent grade hydrochloric acid and S7.10.1 A corrosion ratio of 1.25 or less for the thinnest50 % water. section of the weld is permissible. Other criteria, such as a ratio S7.3 Approximately 2-in. long samples shall be prepared of 1.00 or less, may be speciﬁed upon agreement between thefrom a production length of tubing. Shorter, 1-in. samples may producer and the purchaser.be used for small diameter (1/2-in. and below) tubing. Split thesample longitudinally to allow for easy micrometer measure- S8. Special Applicationsments. The sample may be one piece which contains the weld S8.1 For special applications, such as hydraulic expansionand at least 90° of base-metal to one side of the weld. of tubes into tube sheets, there shall be no dimensionalAlternately, the sample may be two separate pieces with one indication of the weld. Tubes ordered to this requirement shallcontaining the weld and a similar size section from the balance bear the additional marking of NB. 9
A 249/A 249M – 04S9. Additional Testing of Welded Tubing per ASME S9.3 The test methods described in the supplement may not Request be capable of inspecting the end portions of tubes. This S9.1 Each tube shall be subjected to an ultrasonic inspection condition is referred to as end effect. This portion, as deter-employing Practices E 273 or E 213 with the rejection criteria mined by the manufacturer, shall be removed and discarded.referenced in Speciﬁcation A 1016/A 1016M. S9.4 In addition to the marking prescribed in Speciﬁcation S9.2 If Practice E 273 is employed, a 100 % volumetric A 1016/A 1016M, “S9” shall be added after the grade desig-inspection of the entire length of each tube shall also be nation.performed using one of the nondestructive electric tests per-mitted by Speciﬁcation A 1016/A 1016M. SUMMARY OF CHANGES Committee A01 has identiﬁed the location of selected changes to this speciﬁcation since the last issue, A 249/A 249M – 03a, that may impact the use of this speciﬁcation. (Approved May 1, 2004)(1) Added UNS 35045 and UNS 38815 Chemistry to Table 1. (3) Added UNS 35045 and UNS 38815 Tensile and Hardness(2) Added UNS 35045 and UNS 38815 Heat Treatment Requirements to Table 4.Requirements to Table 2. Committee A01 has identiﬁed the location of selected changes to this speciﬁcation since the last issue, A 249/A 249M – 03, that may impact the use of this speciﬁcation. (Approved December 1, 2003)(1) Added heavily cold worked (HCW) processing in Para- (2) Increased size range to 12 in. [304.8 mm] in Paragraph 1.3.graphs 1.1, 3.1.2, 5.1, 5.1.2, 13.8, and 19.1. Committee A01 has identiﬁed the location of selected changes to this speciﬁcation since the last issue, A 249/A 249M – 02, that may impact the use of this speciﬁcation. (Approved October 1, 2003)(1) Clariﬁed ordering requirements to include purchaser’s (3) Added 14.2 to provide additional requirements for weldresponsibility. thickness.(2) Replaced unclear wording in 7.1 and 8.1. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website (www.astm.org). 10